Before revision: Comparison of properties URL URL URL URL URL Victus URL ArmorAnnouncedFeb 2008Jan 2012Jan 2013Nov 2014Jul 2016Aug 2016Jul 2018Jul 2018Aug 2019Jul 2020Nov 2022Jan 2024Density in g/cm32.422.392.422.432.42.42.41Young's Modulus in GPa71.57065.877777779Poission's Ratio0.210.220.220.210.210.210.22Shear Modulus in GPa29.628.52631.731.931.432.2Vickers Hardness (200g load): Unstrengthened in kgf/mm2534555489559611590595Vickers Hardness (200g load): Strengthened in kgf/mm2649653596608678651670Fracture Toughness in MPa m0.50.680.660.670.690.70.760.82Coefficient of Thermal Expansion (0–300 °C) in 10-7/K81.475.886.978.875.272.558.8 Related products On October 26, 2011, Corning announced the commercial launch of Lotus Glass, designed for OLED and next-generation LC displays.
After revision: Comparison of properties +Generation1245Corning Gorilla Glass PI Sheet corning.comSR+6Corning Gorilla Glass PI Sheet corning.comDX/DX+3+VictusCorning Gorilla Glass Victus PI Sheet corning.comVictus 2Corning Gorilla Glass Victus 2 PI Sheet corning.comArmorAnnouncedFeb 2008Jan 2012Jan 2013Nov 2014Jul 2016Aug 2016Jul 2018Jul 2018Aug 2019Jul 2020Nov 2022Jan 2024Density in g/cm32.422.392.422.432.42.42.41Young's Modulus in GPa71.57065.877777779Poission's Ratio0.210.220.220.210.210.210.22Shear Modulus in GPa29.628.52631.731.931.432.2Vickers Hardness (200g load): Unstrengthened in kgf/mm2534555489559611590595Vickers Hardness (200g load): Strengthened in kgf/mm2649653596608678651670Fracture Toughness in MPa m0.50.680.660.670.690.70.760.82Coefficient of Thermal Expansion (0–300 °C) in 10-7/K81.475.886.978.875.272.558.8 Related products On October 26, 2011, Corning announced the commercial launch of Lotus Glass, designed for OLED and next-generation LC displays.